Download presentation

Presentation is loading. Please wait.

Published byAvery Denman Modified over 2 years ago

1
Section 1 Concrete Mix Design 1

2
CONCRETE INGREDIENTS Aggregates Fine Coarse Portland Cement (PC) Water Admixtures Paste = PC + Water Mortar = PC + Water + Fine aggregate Concrete = PC + Water + Coarse and Fine aggregates 2

3
DENSITY AND UNIT WEIGHT density = = m / V unit weight = = W / V specific gravity 3

4
WATER CONTENT Oven Dry Air Dry SSD Moist 4

5
WATER-CEMENT RATIO 5 historical records of strength are used to plot f c vs. w/c f cr w/c Ratio 5

6
MOISTURE ADJUSTMENTS EXAMPLE The following preliminary concrete mix has been designed assuming that the aggregates are in oven-dry condition. Water 305 lb/yd 3 Cement 693 lb/yd 3 Coarse aggregate (SSD) 1,674 lb/yd 3 Fine aggregate (SSD) 1,100 Ib/yd 3 The properties of the aggregates are: CAFA Absorption (moisture content at SSD) 0.5% 0.7% Moisture content as used in mix 2.0%6.0% The amount of water (lb/yd 3 ) that would be used in the final mix is most nearly: (A) 206 (B) 222 (C) 305 (D) 388 6

7
MOISTURE ADJUSTMENTS EXAMPLE The moisture content of each aggregate includes: (1) water that would be needed to bring aggregates to SSD condition (the absorbed water) and (2) the excess water that is free to add to the mix water. Since the as-used moisture content is greater than the absorption for each aggregate, each aggregate contributes the excess water to the mix, thus reducing the water that must be added to mix. The water added to the mix is the water computed for oven-dry aggregates (305 Ib/yd 1 ) plus the excess water in each aggregate. Final water 305 -[(2.0% -0.5%)/100] x 1,674 -[(6.0% -0.7%)1100] x 1,100 = 221.61b/yd 3 THE CORRECT ANSWER IS: (B) 7

8
OVERDESIGN Design engineer specifies a strength of concrete used for design calculations – f c Concrete strength is variable Material engineer designs concrete so only a small proportion of the concrete will have a strength less than the strength assumed by the design engineer. 8

9
STRENGTH REQUIREMENTS Normal distribution Increasing strength Average strength ½ the concrete has a strength less than average Standard deviations 1.34s f cr = f c + 1.34s f cr – average strength for mix design Adding 1.34s to f c – 90% of the concrete will be stronger than specified strength f cr fcfc 9

10
STRENGTH REQUIREMENTS f cr = f c + (1.34 s) when s < 500 psi If s > 500 psi : f cr = f c + (2.33 s) - 500 psi s = standard deviation of f c for a particular mixing plant If s is based on fewer than 30 samples, then the standard deviation of the population is underestimated 10

11
Section 2 Asphalt Mix Design 11

12
SUPERPAVE & PERFORMANCE GRADE BINDERS After the Strategic Highway Research Program (SHRP) Superpave (Superior Performing Asphalt Pavements) mix design method for asphalt concrete performance grading method for asphalt binder specification 12 Mamlouk/Zaniewski, Materials for Civil and Construction Engineers, Third Edition. Copyright © 2011 Pearson Education, Inc.

13
Control specific distresses Rutting Fatigue cracking Thermal cracking Specific aging conditions Unaged Construction Long term 13 PERFORMANCE GRADE BINDER CHARACTERIZATION Mamlouk/Zaniewski, Materials for Civil and Construction Engineers, Third Edition. Copyright © 2011 Pearson Education, Inc.

14
SUMMARY 14 Fatigue Cracking Rutting RTFO Short Term Aging No aging Construction [RV] [DSR] Low Temp Cracking [BBR] [DTT] PAV Long Term Aging

15
15

16
SUPERPAVE BINDER SELECTION EXAMPLE Average 7-day Maximum Pavement Temperature = 63 ° C Minimum Pavement Temperature = -23° C Superpave Binder Grace PG-64-22 16

17
PROPERTIES EVALUATED FOR HMA MIX DESIGN Percent G mm at N initial Voids in total mix VTM – air voids embedded in the HMA 4% for mix design 4 to 8% for construction >2% over the live of the pavement Voids in the mineral aggregate VMA – measure of the asphalt film thickness – controls the minimum asphalt content Criteria is a minimum Decreases as the nominal maximum aggregate size increases Large aggregates have less surface area to coat Voids filled with asphalt VFA – percent of the VMA filled with asphalt Criteria is a range In mix design controls the maximum asphalt content Dust to binder ratio D/B – controls dust in the mastic of dust & binder 17 Mamlouk/Zaniewski, Materials for Civil and Construction Engineers, Third Edition. Copyright © 2011 Pearson Education, Inc.

18
18

19
Section 3 Test Methods 19

20
MECHANICAL TESTING OF STEEL Tension Test Determine yield strength, ultimate (tensile) strength, elongation, and reduction of area (Poisson's Ratio) Plate, sheet, round rod, wire, and tube can be tested Typical specimens are round or rectangular 20

21
SLUMP Workability is measured by slump test fill a cone in 3 layers, 25 rods each layer lift cone off and measure distance it slumps from original height 21

22
AIR CONTENT TEST FOR FRESH CONCRETE Measures total air content (entrapped and entrained) Only entrained is good but we can't tell the difference from this test 1)Pressure Method 2)Volumetric Method 3)Gravimetric Method 4)Chase Air Indicator 22

23
TESTING OF HARDENED CONCRETE Compressive Strength (f c ) Test Most common test by far (even more than slump) 2:1 cylinders cast in 3 layers rodded 25 times each layer and cured at 95% humidity Or specimens are cored from structure 7 day = 60% of 28 day and 28 day = 80% ultimate strength Typical compressive strength is 3,000 - 6,000 psi 23

24
Split Tension Test To measure tensile strength about 10% of f' c 24

25
Coarse aggregate material retained on a sieve with 4.75 mm openings Fine aggregate material passing a sieve with 4.75 mm openings Traditional Maximum aggregate size – the largest sieve size that allows all the aggregates to pass Nominal maximum aggregate size – the first sieve to retain some aggregate, generally less than 10% 25 AGGREGATE SIZES 4.75mm 1 #4 sieve = four openings/linear inch

26
Resist load damage During construction Traffic loads LA abrasion test TOUGHNESS & ABRASION RESISTANCE Prepare sample Minimum mass original Specified gradation Charge drum w/ sample Steel spheres 500 revolutions Sieve 26

27
Section 4 Properties of Aggregates 27

28
28 Bone dry – dried in oven to constant mass Internal impervious voids Air dry – moisture condition state undefined Saturated surface dry – moisture condition state undefined Moist – moisture condition state undefined Voids partially filled WsWs WmWm W SSD =W s +W p WmWm Free moisture Moisture contentAbsorptionMoisture content Absorption is the moisture content when the aggregates are in the SSD condition Free moisture is the moisture content in excess of the SSD condition. A Percent free moisture = M - A Important for proportioning concrete negative free moisture – aggregates will absorb water positive free moisture – aggregates will release water Aggregate Moisture States

29
SPECIFIC GRAVITY The mass of a material divided by the mass of water whose volume is equal to the volume of the material at a specific temperature, or G = / w w = density of water at specified temperature @ 4 C, w is: 1000 kg/m 3 = 1 g/ml = 1 g/cc 62.4 lb/ft 3 (remember to stay consistent with force and mass units for measurements and the issue of force and mass will go away as G is a ratio) 29 Mass Solid Volume Mass Water Volume G =

30
30 Coarse Aggregate Specific Gravity by the Book (ASTM C127) Dry then saturate the aggregates Dry to SSD condition and weigh Measure submerged weight Measure dry weight

31
31 Types of Gradation on 0.45 Power Graph

32
Section 5 Engineering Properties of Metals 32

33
33 Typical Stress-Strain Behavior of Mild Steel - is linear elastic up to proportional limit. Then non-linear elastic up to elastic limit = yield point = strain increases at constant stress. Then plastic deformation until failure.

34
EFFECT OF CARBON ON MECHANICAL BEHAVIOR 34 Structural Steel 0.12 to 0.30

35
CONSTRUCTION USES OF STEEL Structural steel plates, bars, pipes, structural shapes, etc. Cold formed steel studs, trusts, roofing, cladding Fastening products bolts, nuts, washers Reinforcing steel rebar for concrete Miscellaneous forms, pans, hardware, etc. 35

36
ALUMINUM Primarily used for containers, packaging, aircrafts, and automobiles. In civil projects, primarily used for architectural and finishing elements like doors, windows, and siding with a small amount used for electrical wiring. Not used extensively for structural members: expense strength and ductility coefficient of thermal expansion 36

37
Most plentiful metal on earth One-third the density of steel High strength-to-weight ratio Good thermal and electrical conductivity Anodizing or hard coating for protection Weldable alloys Easy to recycle Corrodes slightly but does not rust High reflectivity Can be die cast Easily machined Nonmagnetic Nontoxic 37 ALUMINUM ADVANTAGES

Similar presentations

© 2017 SlidePlayer.com Inc.

All rights reserved.

Ads by Google